electronic structure of cobalt nanocry stals suspended liquid /67531/metadc896131/...آ electronic...
Post on 09-Jul-2020
Embed Size (px)
Electronic structure of cobalt nanocry stals suspended in
Hongiian Lid, Jinghua Guo2-*, Yadung Yid , Anheas Augustss~n~-~, Chungli Dong? Joseph
Nwdgren', Chinglin Chung5, Paul A1ivisatoslo3,', Geoff Thorn ton7, D. Frank Ogletreet', Felix G.
Rcquejo', Frank de Goo?, Miquel SaherontJ7*
Materials Sciences Division, Lawrence Berkeley National Laboratory, BerkeIey , CA 94720 1
'Advanced Llght Source, Lawrence Berkeley Nationd Laboratory, Berkeley, CA 94720
The Molecular Foundry, Lawrence Berkeley National Laboratory, Berkeley, CA 94720 3
4Department of Physics, Uppsala University, Box 530,751 21 Uppsala, Sweden
'Department of Physics, Tamkang University, Tamsui, Taiwan 25 1, R O C
Department of Chemistry, University of CaIifornia, Berkeley, CA 94720 6
'London Centre for Nanotechnology, Chemistry Department, University College London WClH OM,
'Departamento de Fisica, FCE, UNLP - INETA (CONICET). Argentina
?lkpartment of Chemistry, Uwecht University, The Netherlands
c (MS) and jguo'@lbl.E (JHG). ._ . CORRESPONDING AUTHORS FOOTNOTE: m W m
Y. Yin is now at the Department of Chemistry, University of California, Riverside.
ABSTRACT: The electronic structure of cobalt nanocrystals suspended in liquid as a function of size
has been investigated using in-situ x-ray absorption and emission spectroscopy. A sharp absorption peak
associated with the ligand molecules is found that increases in intensity upon reducing the nanocrystal
size. X-ray Raman features due to d-d and to charge-transfer excitations of ligand molecules are
identified. The study reveals the local symmetry of the surface of E-CO phase nanocrystals. which
originates from a dynamic interaction between Co nanocrystals and surfactant + solvent molecules.
KEY WORDS: Co Nanocrystals: resonant inelastic x-ray scattering: Co LZ3 x-ray absorption and
Advances in the synthesis of particles of nanometer dimensions. narrow size distribution and
controlled shape have generated interest because of the potential to create novel materials with tailored
physical and chemical properties [ 1-31. New propertics arise from quantum confinement effects and
from the increasing fraction of surface atoms with unique bonding and geometrical configurations. Co
nanocrystals display a wealth of size-dependent structural, magnetic, electronic. and catalytic properties.
The challenges in making isolated Co nanocrystals are to overcome the large attractive forces between
the nanoparticles, due to surface tension and van der Waals interactions. that tend to aggregate them.
Using appropriate surfactants however. Co nanocrystals could be grown with controlled shapes and
sizes: either spheres or disks in a surfactant mixture [3-51. I t was found that disks of hcp-Co are
obtained in a binary surfactant mixture at early times after injection of the precursor. and spontaneously
transform to the more therniodynamically stable spheres of E-CO [q after heating for a sufficient period
A fundamental understanding of the growth and properties of the nanocrystals would greatly benefit
from a detailed information of their electronic structure as a function of size and of the presence and
nature of the molecules bound to their surface. Because the Co nanocrystals are extremely reactive and
oxidize easily it is important to use techniques that can interrogate the particlcs in their growth
environment so that their electronic and chemical structurc can be followed during growth and during
catalytic r e x tions.
We report an electronic structure study of Co nanocrystals with a narrow-size distribution suspended
in 1,2-dichlorobenzene (C,H,CIJ using in-situ photon-in/photon-out spectroscopies. including x-ray
absorption (XAS) . x-ray emission (XES) and resonant inelastic x-ray scattering (RIXS) [8.9]. These
techniques are element selective as they involve core atomic levels and thus can probe the local
electronic structure of selected species in a complex system [lo-121. We found particle size effects
arising from interactions with surfactant and solvent molecules at the particle surface.
Cobalt nanocrystals were synthesized by decomposing the carbonyl precursor Co2(CO),. in 1,2-
dichlorobenzene at a temperature around its boiling point (-182 "C) [3-51. Oleic acid.
CH,(CH2),CH=CH(CH2),C021-I. and trioctylphosphine oxide. (CH3(CHd,),P=O (TOPO). were used to
control the growth and to provide a protective surfactant capping. I n a volumz of 18 ml solution the
amount of TOPO was 1 g. The size of Co nanocrystals depends mainly on the amount of oleic acid.
while TOPO has a much weaker interaction with thc cobalt surface. Monodisperse Co nanocrystals with
sizes of 3, 4. 5. 6. and 9 nm (* 0.65 nm) were prepared by simply adjusting the amount of oleic acid
used in the synthesis. The size of the nanocryslals was determined by transmission electron microscopy
(TEM). Samples of liquid suspensions were encapsulated in a small cell inside a glove box under argon
gas before transfer to beamline 7.0 the Advanced Light Source for x-ray spectroscopic experiments [ 131.
The cell was sealed with a silicon nitride window 100 nm thick . Incident and emitted x-ray
photons penetrated through this window. The x-ray absorption spectra werc recorded in total
fluorescence yield mode using a channeltron. X-ray emission spectra were obtained using a high-
resolution grazing-incidence grating spectrometer. The energy resolution was 0.2 eV for XAS and 0.7
eV for XES measurements.
The Co L-edge XAS of nanoaystals are shown in Figure 1, along with Co metal, CoCI,, Co,O, and
COO reference spectra. The spectra contain two regions separated by 16.0 eV due to the core-level spin
orbital splitting of 2p,, and 2p,,. The high branching ratio of LJ(L+L,) in the COO spectrum indicates
a saturation effect due to the Iluorescence-detection method, and for that reason the profile of L,-edge is
used for comparison. The saturation effect is not a significant problem for Co nanocrystals as they are
dispersed in the suspension. The most notable feature in the spectra of the Co nanocrystals is the new
absorption peak. A2. at -6 eV above the main absorption edge that is absent in the Co metal. COO.
Co,O, and CoC12. Since the precursors in the synthesis materials contain only the elements Co. C. 0. C1.
no other absorption lines are expected near the Co L-edges.
We investigated the origin of the A2 peak using the x-ray emission Spectrometer to measure XAS
spectra in partial fluorescence-detection mode. No emission changes associated with this peak were
observed within a window of 50-100 eV centered at the Co L-edge (750 eV), 0 K-edge (525 eV). C
K-edge (275 eV) or C1 L-edge (I70 eV). Thus the fluorescence yield of this peak must be due to
photons with energy below 120 eV. which are detected by channeltron but not the spectrometer. As
we discuss next, we believe that this peak is due to a metal-to-ligand charge transfer (MLCT) to
unoccupied ligand orbitals involved in T[: back-bonding to the Co metal.
The first discussion on x back-bonding in metal L-edgc XAS was given in a study of bimetallic
cyanides of the Prussian blue family [ 1.51. A similar absorption satellite was found for K,Ni(CN), in
comparison with Ni metal or NiO systems, where MLCT transitions to unoccupied ligand orbitals were
identified 116, 171. A similar MLCT feature was observed in KjCo(CN), that adds supports our
assignment [ IS]. The A2 satellite peak in figure 1 is then assigned Lo MLCT transitions between Co and
the oleic acid or 1.2-dichlorobezene. The MLCT satellite peak starts to appear in the nanocrystals of 9
nm and shows an increasing intensity when the diameter decreases. as expected from the increasing
proportion of Co-surfactant molecular interactions.
We can exclude residual unreacted Co carbonyls as contributing to this peak since they should be
preseni i n sirnilar amounts in [he Co nanocrystal suspensions with diameters 3 n m to 9 nm. Also, the
metal carbonyls do not have a strong peak at energies above the L, (and L, edge). :IS shown for example
in the spectra of Mn,(CO),, measured by Ruhl and tlitchcock [ 191. This suggests that the CO ,7: orbitals
have a different energy ordering with respect to the 3d-band that seems not to yield an additional peak:
probably the CO TC* peaks are mixed within the L edge multiplet. This is also seen in heme-like
complexes. as discussed by Hocking et al. .
Figure 2a shows the RIXS spectra from 6-nm nanocrystals recorded at the selected energies indicated
by arrows in the U S . The intensity has been norrnalized to the incoming photon flux. The spectra
comprise three contributions: normal x-ray emission, elastic. and inelastic x-ray scattering. Normal x-
ray emission is dominant at excitation well abo\e the Co L-edge absorption threshold. The normal
emission appears at constant photon energy, 778 eV for L; edge (indicated by dash line). and
independent of chan